University of Warwick institutional repository: http://go.warwick.ac.uk/wrap
**A Thesis Submitted for the Degree of PhD at the University of Warwick **

http://go.warwick.ac.uk/wrap/73652

This thesis is made available online and is protected by original copyright. Please scroll down to view the document itself.

WAVE PROPAGATION IN NEGATIVE RESISTANCE MEDIA

A thesis submitted by

A. C. Baynham, B. So.

for the Degree *ot* Dootor *ot* Philosophy
at the University *ot* Warwiok, Coventry,

Preface

The work described in this thesis was carried out at the

Royal Radar Establishment, Malvern, between early 1969 to early 1971. Supervision during this period was shared by Professor P. N. Dutcher at the University of Warwiok and Dr. E. G. S. Paige at the Royal Radar Establishment.

Three papers have been published by the author upon the work described here, and a further paper 1s in the oourse of preparation. Those already published are I

Wave Propagation in Negative Differential Conductivity Media I n-Ge A.C. Daynham, I.D.M. Jnl.Res. and Dev.

### 1l,

No.5,56$-572, (Sept.1969)

Emission of T.E.M. Waves Generated within an n-Ge Cavity A. C. Baynham, Eleot.Lett. ~, No.10, (4 May 1970) A New Mode of Miorowave Emission from GaAe

A. C. Baynham, D. J. Colliver, Elect. Lett. ~, No.16 (6 August 1970)

The latter paper is the only artiole published or to be published with a joint authorship. Mr. Colliver's contribution to the work described

in that paper was a valuable assistanoe in fabrioation of alloy contacts upon GaAs. The remaining work described here is also original with the exoeption of that reviewed in Section 1 and those portions 1n subsequent seotions where acknowledgments to other workers are specifically inoluded.

The author would like to thank both Professor Butcher and

### Dr.

Paiee for their oonstant interest and numerous helpful discussions. He would also like to thank the Ministry of Technology for their financial support during the course of this work, and Mrs. Bartlett for her careful typine of the thesis.Published by kind permission of the Controller, H. ~. S.

### o.

-1-ABSTRACT

Wave Propap;ation in Negative Resistance Media

When an e1eotromagnetio wave enters a medium having an effective negative resistanoe, it may be expected to grow spatially. The conditions under which such growth may be observed are examined, and an experimental regime ohosen where it should be possible to observe these effeots.

Suoh observations can throw light not only upon the negative resistance travelling wave amplification process, but also upon the transport process giving rise to the host negative resistanoe. The experimental work is therefore divided between a stu~ of a new negative differential

conductivity prooess recently discovered in n-Ge and 8 stu~ of the

negative resistanoe travelling wave amplification prooess in GaAs.

The diagnostio measurements upon n-Ge provide new data relating to the negative resistanoe process in that material~ data such as the maximum negative slope mobility of 300 cm2/V.seo. at 77°K (B / / <100» the threshold eleotrio field for

### N.D.C.

of 2.95 XY/cm.### (E //<100»),

and the oeiling frequency of### 5

GHz beyond whioh N.D.C. dissappears, all*ot* which have been subsequently corroberated by other workers.

Observations of the emission speotrum from GaAs, when the amplified eleotromagnetio wave begins to experienoe round trip gain within the specimen oavity, have allowed some fairly detailed disoussion to be

undertaken concerning the nature of the emission process, which rely upon
careful measurements *ot* the speotral power and line width. Although the
maximum pulse power observed of

### 4

mW is low, such observations of emissiondo provide

### a

new meohanism by whioh miorowave power may be extracted from a suitably biased material having a negative differential oonductivity.,Finally, attention is diraotad towards some potent1all1 profitable areas for future work.

-11-Index:

Section 1

Preface Abstract

Index

HISTORICAL SURVEY I The Concept of Wave

Propagation in Negative Resistance Media, and a Desoription of Suitable Media.

1.1 The Quest for Solid State Travelling Wave

P<lce i 11 iii 1 2 Amplification.

1.2 Negative Differential Conduotivity in

Gallium Arsenide.

4

The Eleotronio Transport Process The Maoroscopio Consequenoes of Negative Differential Conduotivity.

1.3 Negative Differential ConduotivitY,in n-type 16

1.2.1 6

1.2.2 _{11}

Germanium.

Seotion 2 Wave Propagation in Conducting Media. 2.1 T.E.M. Wave Propagation in an Infinite

Unif'orm Medium.

2.2 Finite Speoimen Geometry

2.2.1 Finite Speoimen Geometry in the

### 26

21

30 )0

2.2.2

Direotion of \1ave Propagation.

Finite Specimen Geometry, in the

### 35

Direotion of' the Applied Eleotrio Field.Wave Polarisation

Choice of Frequenoy of Operation

*"*

40

### 42

-111-Section

### 3 .

Measurement of Negative Mobility by a Bridge Teohnique.3.1 n-Typa Germanium

### 48

### 49

3.2 Conoept and Planning of Experimental Regime. 49

3.2.1 Stability of Speoimen.

### 50

3.2.2 Non-uniformity of Biasing Eleotrio Field. 52

3.2.3 Frequenoy Limit. 54

3.3 Summary of Experimental Constraints Leading

### 55

to a Finalised Experimental Soheme.### 3.3.1

Miorostrip Transmission Line. The Experimental System. Specimen Problems### 56

### 51

58 59### 59

Section 4 3.3.4 Measurement. ·Analysis of Results.Observation of Emission of T.E.M. Waves Generated within an n-Ce Cavity and their Diagnostio Potential.

4.1 Experimental Concept. 4.2 Experimental System 1.

4.2.1 Bright-up Teohnique.

4.2.2 The Measurement and Results. 4.3 Experimental System 2.

64

Integrating "Latch and Hold" Deteotion. The Measurement and Results.

### 65

### 65

### 65

### 66

68 68### 69

Importanoe of Free Carrier 11

Concentration and Speoimen Geometry.

Threshold Eleotrio Field.

### 78

Temperature Dependenoe.

### 19

Crystallographio Orientation Dependence.

### 79

-1v-Section 5 Observation of Emission of T.E.M. Waves

_{82}

Generated within a GaAs Cavity, and some
Charaoteristios of the Emission Speotrum.

5.1 Choice of Experimental Regime. 83

Speoimen Stability. 83

Non Uniformity of Biasing Eleotrio Field.

### 85

Frequenoy Limit. 86

Speoimen Impedance 86

5.2 Observations of Microwave Emission from GaAs. 86

### 5.3

Conoluding Comments.### 96

Section 6 The Mechanism of Microwave Generation I The Form

### 99

of the Emission Spectrum.

6.1 Theoretical Relationship of Spectral Width 100 and Power.

6.1.1

6.1.2

Emission Speotrum from a Linear Arr~ _{100}
of Noise Sources within a Cavity.

The Power Speotrum from a Noise 103 Amplifier.

6.2 Experimental Investigation of the Nature *ot* 112
the Emission Speotrum.

6.2.1

6.2.2

Demonstration of Eleotrio Field _{112}
Dependenoe of Emission Frequenoy.

Demonstration of Frequenoy Sweeping with a Hi&l Field Pulse and Power

116

Measurement.

Intrinsio Speotral Line Width. _{122}
6.3 Summary of the Form of the Emission Spectrum. 123

-v-Observations of Microwave :Elnissionfrom GaAs

Samples which are Space Charge and

Eleotromagnetioally Unstable.

7.1 Experimental Teohnique and Results. Section 7

Seotion 8 Conolud1ne Remarks.

Appendices I, II and III

### -vi-•

126

127

**1.** HISTORICAL stmVEY : ThA Concept of"WrtVO Propt'.cation
in Net~ntive Resistance !.!edia, fI.ndt:l. Description of

Suit::l.ble~.!edi~

In this section both the backeround information and the direction of thought which has stimulated the present work is

1.1 The ~lest for Solid State Travellins Wave Amrlitication

For a number of years now there has been a preoccupation amonGst
many workers with the hope that it might fall to them to disoover the
high frequency solid state amplifier which would finally replace the
travelling wave tube *(~,1T).* Not unnaturally, most of the thuucine
has been along the lines of a direct analogue to tho ~,'lT. Attention
has been focused upon semioonduotors beoause of the high eleotron drift
velooities which can be achieved whilst maintaining the aocompanyinG
power dissipation within acoeptable bounds. The host of waves known
to propagate in semiconduotors have each, it would seem, been subjected
to high electric fields in the search for amplification. Helicon waves~1)
AlfV6n waves(2), helical waves(3), space charge(4) and dipolar space

charge waves(5), spin waves(6), acoustic(1) and optic Phonons(8), have all been studied during this searoh. Sucoess has however been minimal; the only real suocess being with the acoustio amplifier, and even here upper frequenoy limits are so low that transistor amplifiers still offer

superior performance.

In some cases the reason for this lack *ot* suocess can be hinted at.
Most of the drift/wave interactions have a gain threshold which is

determined by the relative magnitude of the eleotron drift velooity and the phase velocity of the wave as in the TWT. However many of the waves cited (plasma waves in particular) aocelerate in the presenoe of a

biasing eleotrio field. ConsequentlY any attempt to achieve synchronism between drifting eleotrons and an aooompanying wave may be unexpeotedly difficult, necessitating very high power dissipation within the

semiconductor sample. Even if, at this ste·se, synohronism is achieved, the free carriers have usually entered the hot electron regime, and the

-2-VELOCITY FIELD DIAGRAM FOR NEGATIVE CONDUCTIVllY (UPPER) AND

NEGATIVE DIFFERENTIAL CONlYJCTIVITY (LOWER) MEDIA

**ELECTRON**

**VELOCITY A**

**ELECTRIC**

**FIELD**

**ELECTRON.**

**VELOCITY:**

**FIG**

**I**

**IT**

### 1

### ~1

### E

-simple oold eleotron model, so often employed in this work, is invalid.
It was within this context of diseillusionment with synchronous
instability that the present work oommenced. _{One was forced to ask if}
an alternative class of instability could be conceived of, and immediately
the possibility of wave propacation in a negative resistance medimn was
introduced. _{It 1s this intuitively} _{obvious amplification} _{mechanism} _{with}
which we shall be concerned here. _{A} _{fundamental} _{difficulty} _{is, of course,}
encountered when a suitable total negative resistance medium is soueht.
(See upper diagram in Figure 1). So far as the present author is aware ,

the only such mechanism, proposed by Stocker(9), haa only recently been (9a)

demonstrated experimentally • However, a number of materials are now
known which exhibit negative differential conductivity. _{(Lower}

diagram in Figure 1). It was therefore proposed that one of these

materials be biased into their region of negative differential conductivHy, when an incident wave will behave as if entering a material having a

total negative conductivity. (This statement is examined in detail in

Seotion 2). The lower portion of Figure 1 shows sohematically how a suitably polarised osoillating field may be viewed as superimposed upon the biasing field.

Similar lines of thought have been pursued by other workers. For ( 10)

example, Midford and Eowers have launched a transverse electro-magnet ic wave through a silicon Impatt device, and Rob Inson and Kino (11 ) have launohed space charce waves in a Gunn device which was stable acalllst domain formation. Each of these sets of workers have achieved eain,

and the space oharge wave amplifier ha.s now been studied extensivel}12,13,14). The present work has followed an intermediate path, fOcussinG

attention upon the propagation of a transverse eleotrio wa.ve within two

### -3--

### __

..### _--'zl

### _./'/

0### t

(i### n

0 t.;,J 4'1 ::> ENERGY V_{A}

### ..,..

### L

cl ~I_{CRYSTAL}< MOMENTUM

### ~I

Cl lA.. ::x: u### ._

Cl: -; 0 UJ UI 41( cc### ....

ELECTRON VELOCITY### .

0-Cl N liE> KT### __ W __

### ---J

FIG.20

'\

CONDUCTION BAND ENERGY MINIMA

(j)

ELECTRICFiElD

FIG.2b

:) ELECTRON VELOCITY - FIELD CURVES CHARACTERISTIC OF

~ ELECTRON IN MINIMA {j} AND Oi) TOGETHER WITH A

DOTTED COMPOSITE CHARATERISTIC

A-4 SHEEr

### '---

### --..----

---_...---different materials (n-Ge and GaAs) which both exhibit a negative
differential conductivity. _{It is shown} _{in} _{subsequent} _{seotions} _{that}
wave amplifioation oan be obtained in both materials. _{In} _{addition}
osoillation is demonstrated under suitable feed-baok oonditions, and it
is shown that the propagating transverse eleotromagnetio wave may be
employed as a diacnostio tool with whioh to stu~ the negative

differential oondu·otivity phenomenon.

1.2 Ner,atlve Differential Conductivity in Gallium Arsenide

In 1961 Ridley and Watkins(15) first disoussed the possibility

of negative resistanoe effects occurring in semio?nduotors. The thoughtl3 of these two authors together with those of Hilsum(16) oonoerning the application of suoh effeots laid the foundation for observations of miorowave emission to be made by Gunn(11) a few years later.

The proposed negative resistance meohanism was based upon a
combination of features of the eleotronio energy band struoture whioh
oan ooour in semiconducting materials. Attention was fooused upon the
details of the behaviour of eleotrons in a material having a light m~ss
oonduotion band edge and olose to it, but a little higher in enereY, a
heavy mass minimum ( (ii) in Figure 2A). Eleotrons in the lower light
mass minimum ( (i) in Figure 2A), are then expeoted to exhibit a la.rge
mobility in oomparison to any in the upper heavy mass minimum. Hm./ovor,
the energy separation of the lower and the upper minima *(~t* *)* is to be
such that at room temperature there are few if Rn1 eleotrons in the upper
minimum. Thus at room temperature the observed velooity field curve is
expeoted to be oharaoterisod by eleotrons exolusively oonfined to the
band edge (Figure 213).

As the applied electrio field is increased, the lieht electrons gain energy rapidly from the eleotrio field owinB to their hiGh mobility,

### er:

### f2

UI..1J

### >

W_{....,.}

0

### <!

_{z}

~

_{<t}

### "

0(1)

### "

E*I*

### "

ZI

*-o*

### 0

\

### ,

### 0

### t-

_{U}

### "

### ....

::>Cl### z

### A~tJ3N3

### 0

_{u}

W M

Cl **(l)**

### -"

Z LL/ W

*I* (f)

I

### a:

\ <!

\

### "

_{>}

### L

### ::>

_J

0 ~ _J

E \0('f)

### «

in

### .

(9('f)

### 0

•

### 0

**.11**

(energy/oarrier/ sec •

### fA

E2) and at quite modest eleotrio fields it is possible for the electrons to assume a very hieh mean energy.(15000K) (18) so that, althoueh

### Ll

*E*

»k"T, the electrons may
never-the-less begin to transfer to the upper minimum. Let us assume that at
some defined field strength a oatastrophio total eleotron transfer ocours. Then the observed external velocity field ourve must ohange from that oharacteristio of the light mass minimum ( (i) in Figure za) to one oharaoteristio of the heavy mass minimum ( (ii) in Figure

*ZS).*

The
averl'1,cevelooity-field oharacteristic resul tine from such a transfer is
shown dotted in Figure 2B and is seen to demand a reduction in current
density and therefore a region of finite negative differential
conduotivity (Nne) beyond a threshold field ET' This, then,is the immediate intuitive explanation of the negative differential conductivity to be exploited here, and is seen to be based upon a non-equivalent

intervalley scattering meohanism; the transferred electron mechanism.

### *

GalliUIl Arsenide is one of a number of materials which may be expeoted to have a suitable conduotion band structure for observation of the Ridley-Watkins-Rilsum negative differential resistanoe. As shown in Figure 3, at the oentre of the Brillouin zone we encounter the band edes with a small effeotive mass of 0.061 ID (19) where m is the free electron

o 0

mass. At the edges of the Brillouin zone in the (100) direction there are three further conduction band minima, about'0.35 eV (20) above the

conduotion band edge. These are thought to have a mass of 0.35 m by

o

### ---*

Other materials InP (22), CdTe (23),*~_S,/(114J*

in which the Gunn effect haa been observed are ~" ~ GaAsP (24) alloys and InAs under suffioient ,

uniaxial strain to prevent impact ioniaation(25). In the case of In? it is now proposed that the mechanism is in fact a "three level" variant upon the Gunn effect(26). Never-the-1eas it remains an electron

transfer phenomenon.

comparison with GaP which is a similar material but has the (100) minima at the band edee where they may be readily studied.

When GUl1n first ob served (17) microwave emission frOll GaAs it was not immediately attributed to the transferred electron mechanism. However, there is now no doubt that GunnIs observations are due to

the Ridley-\7atkins-Hilsum mechanism. Overwhelming justification for this identification are for example, in the variations of the threshold field with strain, temperature and alloying, and the class of materials fro~ which precisely similar emission (18) is to be observed.

1.2.1 The Electronic Tra.ns1')ortPJ"ocesa

Rather than folloVi further the historical development of the transferred electron mechanism we set out a more detailed aCOOtD1t

of the relevant principles which underly it. \'10 beein by d.escribine the transport process giving rise to the instability.

It is common to write the drift velocity (v) in tenns of an average over the contributions from various valleys, thus

where

### Pi

is the mobility in the ith valley containi~ ni free electrons, and*E*is the applied electric field intensity.

It 1s the behaviour of the electron system within the ith valley which fixes u...

*v.IE.*

Their behaviour is summa.rized
*13,* 1

•

by the Boltzmann equation. In a multi-valley system this is conveniently written as

e

### .

### -

\ (~fi (k) \) + _ ... )

where f

### Qs,)

is the eleotron distribution funotion in valley i, ~ being the eleotron wave veotor. The second and third termshere describe the effects of intra-valley and intervalley

scattering events respectively, and these remain to be desoribed. We oonsider soattering by phonons first of all. The contribution

~f.'(k)

to L due to eleotron scattering from a state at k to states

~t

### ,

### ,

at all k for which

### k - ~

is equal to the phonon wave-vector is### -2JJ

### -

~, ,t ,*L ,*

f ### <£)

(1 - f(ls. ) 13<1s.,~ ) N f(E(k) - € (5)k .

+

### pr~.

f### Qs,')

(1 - f*<1s.j*

13~.~') 11### d

(E ~) -### €:

### <l') -

### to;

(ls. -### ~'»)

n k ,

In these expressions

*t*

### Ck)

normalised so that*Ifi~)*

the electron distribution function is

d k ...n., number of electrons par unlt

- l.

th fl? • )

volt~e of the crystal in the i valley. B~I ~ is a p~rnmeter

second describes electron transfer from a hisher anerGY state by whioh specifies the strength of scattering between the states at

### ,

k and k. Tha first term on the rieht hand aide describes electron transfer to a higher energy state by absorption of a phonon, the

stimulated and spontaneous phonon emission, the third describes electron transfer to a lower energy state by stimulated and

-7-spontaneous phonon emission and the fourth describes electron transfer from a lower energy state by absorption.

The expression can be approximated to

, "

### ,~

### ,

### - E

(!£ ) - n*W*{J£ -

### 1£ )

### ,

Inthe case of inter-valley scattering all states le lie in a valley which is not equivalent to the one in whf.ch the state k is found, whilst in the case of intra-valley scattering k and

### •

k lie in the same valley.

Intra-valley scatterll1g is dominated in pure materiRl by, polar optic modes at low fields (21) and by acoustic phonons at hiehor fields, the polar mode scattering havine become weak owine to the

### •

large (~ - 1$ ) ranee of ls. vectors now encountered. Phonons which

may provide ~ conservation in intra-valley scattering processes are of oourse those lying near the oentre of the 13rillouin zone where the optical mode energy is approximately independent of the ~ vector and Bii (~~') is knO\7n in this approximation(21). Similarly the

scattering term for acoustic phonon scattering is known under simplifying assumptions of isotropic Valleys(28).

involved in this process is determined by the symmetry of the initial and final states(21a). If the satellite minima are at the edGe of the zone (as is believed to be the case) then the L. O. phonon is involved, whilst, if the satellite valleys lie ''1ithinthe Brillouin Zone both L.O. and L.A. phonon may participate in the scatterine. A similar symmetry ar~~~ent is involved in determinine the domin~~t equivalent intervalley scattering process. Ionised impurity

scattering is weak for inter-valley scattering where the chance

of k vector is large but may be ~nportant for intra-valley scatterinc. It is however commonly neglected unless the material is exceptionally impul'e.

Once the various scattering terms are known, it remains to solve the 1301tzmann equation in the steady state situation where

*( d*

f/ ~ t) • O. It is at this point that the problem becomes
really difficult. The most common simplifyine assumption has beon that electron-electron soattering is dominant, establishing a

displaced Maxwellian distribution function (29) • One then simply solves the equations for the paramet.ara of the distribution functLon,

More recently it has become possible to carry out exact nuraer-Lcat

solutions of the 1301tzmann equation by the Monte Carlo technfque (30) • Here the path of a single eleotron is fol1owed through k space over m~ scattel'ing events. Ey careful "book keeping" of the time spent

in each elemental volume of k space, the electron distribution function and thence the mean electron velocity is thus obtained.

Suffice it to say, that it is possible to obtain the electron distribution function, and the eleotron drift velocity as a ~mction of eleotrio field strength, by a. number of methods. Such

calculations have provided a variety of results. The most recent

-9-If) w > 0::: ::>

### o

0 _J W LL >- 1-u 0 -' UJ > _J <t: U### .._

W a: 0 w y I### .

r### 8

(Y) Cl Z### ...

### «

-c -' Vl <t: <t: I- a z ~w er:_{~}

0 0::: LL W n. x w LL 0 Z 0 If) 0:::

*et*

~
0
u
**....0**X M N 0

**(:>3S/~:))****),,11:)0131\** **1.:JlldO**

ia that of Fawoett et al (31) whioh bears a olose similarity to the

speoimen oontaot vias of gold but separated from the specImon by a experimentally determined velooity field curve as shown in

Figure 4. The experimental results shown in Fieure 4 were obtadncd by a time of flight teOhnique(32). This requires very high

resistivity material. (106 - 108_f.Lcm). The negative

thin film of SiO, whilst the anode was a straight forward N+ tin contact. A short pulse of eleotrons ejeoted by an eleotron beam at the oathode was then timed as it travelled to the anode under

various biasine eleotric field intensities. In this way the electron velocity was obtained as a function of eleotrio field intensity.

'.

These results are probably more reliable than those of a variety of other VJorkers owine to their freedom from interpretative problems. For example, Ounn and Elliott(33) have made a measurement of s~ple

impedanoe in a time short oompared with the dielectric rel~~ation tima. One is however, conoerned to know the response of the hi6hly oonduoting oontact rag ion in suoh an experiment. :F'urthermore, if the theoretioal estimates of the negative mobility are oorrect the measurement was alrea~ too slow by a factor of ten. Thus it ia not surprising that this measurement provided a low apparent negative slope mobility.

In oonclusion then, theoretical estimates of the stutic velocity field oharacteristics have been made which have, by and large, a common starting point, but differ in the means adopted for

eluoidating a final solution. Experimental work, 01'1 the other hand,

has also been performed which furnishes information concerninG this vital N.D.C. characteristio. The best rasul ts of the two disciplincc),

1.2.2 The Ul"croscot':i.cConse('uences of N. D.C.

Our objective in this section is to review contemporary understanding of the macroBconic behaviour of a specimen which has the microsconic differential conductivity discussed in the previous section.

a) S'P~ttialNon Unifomi t,y in Stable Snec1.mens In one dimension Poisson's equation gives

• • •

for n type material. Here n is the local tree electron

concentration,

*e.*

the electronio cha.rge, EL the lattice dielectric
constant, and no is the density of ionized donors.
Looking for a time-independent solution we obtain from the current continuity equation,

*0*

### J/a

x • 0, the resultJ - nev (B) • constant _{• •}

_{•}

Now, clearly, if at all points n • no in equation (1), n, E,

*p*

and
consequently J all become spatially independent to satisfy equation (2).
However, we know that at the contact the field is considerably
below its value in the centre of the specimen. Thus it emerces that, because of the contacts, n cro1not equal no at all points in the specimen and that the boundary conditions therefore playa vital role in determining the behaviour of any specimen. This was pointed out lone ago by Shockley(34) and has been emphasised more

recently by Kroemer(35).

We discuss first of all a sample biased so that at all points within the specimen E

### < ~.

Let us consider a point "A" (Figure 5a) immediately inside the Cathode where the electric field### -11-·_---

### -

---_..- -### ---z

### o

o \oJ VI*I::)*/.-4---_J~

, It .•./ E-c E THRESHOLD

### E 'E-O

### ~/---l

I I I

### I

I II

### I

I### ntN'

I### <,

## 'J

n =no

----,

### "

### .

~ o### :tl

et### ~I

### e

_{::c}u

### ._

a.. -; FIG. 50ELECTRIC FIELD AND FREE CARRiER DISTRIBUTIONS

IN A SAMPLE BIASED BELOW THRESHOLD

Q LIJ ul et cc:

### ...

### I

### e

l### I

### I

*I*

### vt

### I

*/1*

### E •

### "

### ....

,,,/EeO j!(E)-.Y_

I _{I}

### E

I _{I}

I

### I

### nt

### I

### //

### 1///

### n:::no

RR/R3/02619

### ---

-_{829'18:':}

### ---

_{·)00}

_{B 7:.; :-...}

FIG.Sb

ELECTRIC FIELD AND FREE CARRIER DISTRIBUTIONS IN A

SAMPLE OIASED BEYOND THRESHOLD FOR N.D.C.

A<4 SHEET

'---is still increasina in intensity away from the cathode. At this

dE

point - in + ve , and thus from equation (1) n,/ no. In

dx

equation (2) we see that this is an acceptable solution. Substituting (1) into (2) we see that

• • •

### cm

Thus as E increases with distance from the cathode, - decreases 7

dx

and the system rapidly tends to a spatial uniform field distribution with E la EJ

### <

### E.:r

,where EJ is determined by*s -*

no...c.2..*V(E:r).*

We tumour attention now to a sample biased so that a part of the specimen has a field in excess of the threshold field E.r • Consider a point

### ":B"

(Figure 5b) where E /' ~. Here the field, we suppose, is still increasing spatially towards the mean applied field, for it remains necessary that### /

### 1:: •

### i!. -

Total Applied Voltaee •However, in this case, increase of E necessarily now produces a raUir:.:.:

V(E),and the tendenoy to equilibrium with .@ ~ 0 is no longer found.

, dx

In order that *:r* remain oonstant n must rise indioating, with the
aid of equation (1), not a tendenoy to a uniform field distribution,
but a ":run away" situation, in whioh the field inoreases ever more
rapidly spatially. This system is only brouGht under control
when the field enters a positive slope resistance re81011 of the

velooity field oharacteristio at even higher eleotrio field strenGths. This discussion has shown that a stable electrio field

distribution within a sample ha.ving a lI.D.C. oannot be of tho

familiar uniform nature with a droop at each oontact; this is only found in POSltive oonduotivity media. McCumber and Chynoweth (36)

-12-and Mahrous and Robson(37) have both calculated the spatial field distribution. Doth of these authors negleot diffusion end the first authors verify it to be unimportant to the conolusion. At a later stage in this work (See Seotion 3.2.2), it wil1 be

necessary to pursue this oaloulation for both OaAs and n-Ge in order to evaluate the spatial distribution of the free oa.rrier conoentration within the specimen; neither of the foreeoing authors having evaluated this term.

b) The. DeveloEment of' Instfl.bilit,y

In the foregoing discussion a time-independent solution of the ourrent oontinuity equation was specifioally sought. However, this stea~-state distribution will be unstable if a small space

charge fluctuation, generated either by noise within the speclinen or switching transients outside the specimen grows in time. A nu.rnberof estimates of the "amount of negative resistance" which can be tolerated whilst retaining stability have been made.

Perhaps the most attractive is that of McCumber and Chynoweth (36). These authors oalculate the sample impe~~ce using the foreeoing equations and. firid the system unstable if

i) There is a negative resistanoe region within the sample i.e. the dielectrio relaxation time at the biasll1B field ia negative and

ii) The product of the free carrier concentration N end ,sample length L exceeds a critical value (NL ~ C ).

osc

The critical N L produot whioh defines the threshold of temporal instability is now well confirmed by experiment(18), thouGh empirical values of the product tend to be somewhat larger than theory would suggest.

..., .... 0 0 w VI :J

~

**V**

**K**

### r

### ell

v### .

"t 0 0.._{I}

a...
«
### ~\

_{0}U-

_{}>-:c ~ ~ U

0- 0--J

-, W

>

0 ~

LIJ ~

U _{I} ~

« 0 0:: ~

### ,

### \

### ,

I### ,

.### \

### I

I I I### I

_{,}

### 1

I### I

### · I

### I

### I

### ,

I### ,

I### ,

I### ,,

I I I I I I I I### ,

I VP.M**FIG.6**

**CONSTRUCTION** **OF THE** **DYNAMIC CHARACTERISTIC**

**FOR** **STABLE DOMAINS**

**FIELD**

._---'-'

### -

_,--RR/R3/02620

terminal impedance. _{~ley find that a stable sample, may exhibit}

terminal negative differential resistance over a small ra,nceof fre~uencies centred upon the inverse of the electron transit time through the sample. This fact has been exploited by Thim(43) in making a low N L product amplifier.

c) u>,rr~eSir,nal Inst~tbilit,V'

Inunstable s~~ples space charge fluctuations crow up from noise to assume a characteristic large-sienal form. Ridley OS) , who first proposed that the final fonn is a travelling hieh-field

domain, and Kroemer(39) have both contributed ereatly to the

development of our understanding of domains. ~e confine our attention, however, to the final picture which has emerged.

The problem is once again one of solving Poisson's equation together with the current continuity e~uation. Since tho objective is to find the large sienal stable solution of these equations we look for a solution in which the profile of Ridley' a

domain is constant during propagation i.e. such that the hieh field and the accompanying space charge profiles are itmctions only of

(x - v t) • y •

o A suitable chance of variable in the two startine

equations then allows the new variable y to be eliminated yieldinG a differential e~uation relating the field and free carrier

concentration. This equation has been solved by Butcher(40) under the assumption of a field-independent dif~sion constant. It er1orce.] that the velocity of the domain must equal the velocity of tho

eleotrons outsicle the domain, and that the peak domain field is defined by a simple geometrical construction illustrated in

Figure 6. The two shaded areas have to be equal in order that an integral appearing in ~utcher's solution should vanish as required.

### --1

### ---I

z 0 Cl UJ*VI*:::>

*J*

**Eo**~4 ~/ I .' (

,_{,."}" _{Et}

e : '" <+.-ci o.

_{I}

o.
### «

### I

**ER**

### ER

Cl
0::
0
u...
:c
u _{0}
t=

### 0-...,

0 ur U_{I}

### «

Cl: I-n~### o ~---~---~

....---_-,---...-..-.__....### _-

-RR'R3

**/0**

2 621
### ---

_-- .le'" D ~n~():1t-:~

FIG,7

**STABLE** **DOtv1AIN PROFILE**

UJ

### I~

### .

This latter condition clearly defines a "dynamic" charC1.cteristicof

peak domain field versus drift velocity, which is shown dotted in Figure 6.

The picture which we have of the stable domain is
therefore of a hieh field region propagating throuGh a specimen at
the same velocity as the electron system at each side of it. Its
peak field is defined in relation to the electron drift velocity
and field outside the domain. _{The profile of the domain is shown}

in Figure 7. ?oisson's equation olearly demands that the

accompanying space charge modulation should be of the form shown ,'/hieh is the origin of the common terminologyl "dipold'domain.

Domains which approximate to this shape have been seon by Gunn (41) and Heeks(42) using minature capacitative probe techniques. Less direct evidence of the existence of domains ia of course to be found in the very existence of the transit mode of operation of unstable samples. In this mode of operation a "spikey" current wave form is observed under conditions of constant voltage supply, these spikes corresponding to initiation and collapse of domains at

cathode and anode. The separation of the splices is very closely l'elated to the length of the specimen indicating a. tranoit effect.

We include one further consequence of domain

propagation. _{It will be noticed from figure six that when tho·}
current through a specimen biased beyond threshold is increased, the
domain field falls. _{Detailed calculations} _{show that the domain}
potential also falls, when the specimen current is increased, and
that this effect can be stroneer than the positive resistance effect
of the remainder of the specimen yielding a tenninal negative

resistance (21). The ensuing broad-band neGative resistance has been .exploited by Thim (43) as the basis for an amplifier. In that Vlorktl!o

Gunn sample Vias however a local negative resistance circuit elcr.lCnt unlike the work to be described here at a later staee.

**-15-1.3** N.D.C. in n - Ga

In this section we describe those features of the N.D.C. of n - Ge which were known at the time of the commencement of this work. Since that time some further PUblications(52, 53) have appeared which include those of the present author. 'Discussion of this later work io postponed until the final seotions of Chapters 3 and 4 in order that the contemporary work may be treated in context.

The first observations of current instebilities in n - Ge were made by llcCroddy and Nathan (44). These authors found instability under the followinG experimental conditions

a) Lattice temperature below 150K.·

b) Electric field parallel

### <

100') or <.110)- in the zero stress regime.In the

### <

110> orientation it was possible to change the threshold field by applyinB a uniaxial stress also in the### <

110) direotion. Oscillationf'requencies ranged from a few hundr-edMI-Iz to 2.8 CI-Iz,and were characterised. by a threshold NL product for oscillation of 2 :x: 1013 cm-2• Subsequent work by McCroddy has shown that the N.L. product is "j"lellin excess of

2 - 1013 cm-2 " (Private communica.tion).

In seekine the source of these instabilities, Elliott e't a.l(45) . conducted a series of' fast pulse and potential probil1B experiments. The fast'pulse experiments were designed to make an observation of the sample current and applied voltaBe before the electric field non-uniformity ru1d

associated space charce was able to establish itself; that is before a dielectrio relaxation time had elapsed. They revealed a terminal N type negative differential resistanoe, at

### 27°K

and### 77°K

for electric fiolds in excess of 3 F:J/cm, and parallel to a <1007 crystaloerr>.phic axis.owing to limited response of the circuitry employed, this data CruU10t

be regarded as a quantitative measuremerrt of the elect rio field dependence

### *

of the electron dxift velocity. Thus, thi~ measUl'ement establishes the existence of N.D.C., with a tlu'eshold electric f'ield strength of

3 lCV/cm, but does not yield the value of' the negative slope mobility.

Probing experiments(45), were used to Btu~ the spatial field distribution within the sample as a function of' time. Those

### .

indicated the existence of' dipole domains at 21°K which nucleated noar to the cathode and propagated at a velocity of 1.3 - 101 cm 6eo-1 tOVla.rds the anode. This observation is also consistent with the existence of a bulk N.D.C. in n - Ge at 21°K. (electrio field parallel

### <.

100"7 ) thouGhof unknown oris in or magnituue. Measurements of the velocity field characteristic in n - Ga were made by Chang and Ruch(46) using the

"time of flight technique" (41) • In this method the response of a reverse biased Schottky barrier/intrinsic/n - Ge structul'e to a O. 1 x 10-9 sec pulse is studied as a function of time. The pulse introduces a sheet of electrons within the intrinsio layer and as this traverses it, a terminal current flow is observed. The duration of this current 'PUlse is a measure of the electron drift velocity within the intrinsio layer. Knowing the field strenBth within the I layer, the velocity field

relationship is thus obtained.

An N - type N. D.C. Vias observed for lattice temperatures be-tv/eon

330Kand 1300K and for ourrent flow in the <100) direction in the crystal.

At

### 33

0### K

a slope mobility of### 300

cm2/V.seo was evaluated with a thresholdfield of'1.5 rv/cm, in contrast to the threshold of 3 KV/cro observed by

### ---*

A similar experiment was performed in Gallium Arsenide by Gunnand E1liott(45a). They found a velocity field characteristic which is at considerable variance with more recent work of, for example,

Ruch and KU10(45b).

### ---

_{>}

~

### -

>-<..9

0::

### 0

**ltJ**

### ·z

W

**-(**

### OAND

### STRUCTUFH~

### 0:-- ~J-Gc

### 5 ~---~---~~---~---

### ...

### ----.~

### 3

### 2

**4**

**r---2**

### .L

### A

### r

### II

**REDUCED**

**WAVE**

**VECTOR**

**FIG.**

**B**

.'

Elliott et al (45). At

### 79°I(

a "men.sured slope mobili.l.;y of - COcm2/Vsec1lwas obtained for electric fields between 2.2 J!:)J/cmand 4.3 KV/crn.

Howevel', expel'imental uncel'tainties lead the authors to state that they

"cannot ascertain that a negative differential mobility exists around

### 79°K.tt

Again threshold electl'ic fields obtained by these authors sraconsiderably lower than those of Elliott et al(45).

The oonduction band struotul'e of n - Ge is shown in FiGtll'e8.

A uniaxial stl'ess applied to Go in a:tlY direction other than ~ 100~ cauae s splitting of the <111

### >

conduction band minima, which are degenenat o in the absence of strain. Similal'ly, the degeneracy of the hishel'enerrtY

### <

100:> silicon like minima may be lifted by uniaxial stress applied in other than a### <

111)- direction. r.Ieasurements of the trensportproperties of n - Ge under stl'ess may therefore be used to further eluoid.n.tc the distinctive features of the N.D.C. procean, FolloViine this philosophy

Smith, lIIcGroddyand lTathan have studied the current voltage characteristio;] of a nwnber of specimens under a variety of orientations of current end

uniaxial stress (8) • With ourrent flow in the

### <

211~ direct ion end strews a.long the### <

111") dil'ection, for example, the threshold field reduces froman infinite value at zero stress, to a minimumvalue of 0.45 RV/cmDnd then subsequently increases as the uniaxial stl'eSB is steadily inol'easeu.

The effect of hydl'ostatio pressure upon the eleotl'onio ener~r b?nd structure is clearly isotropic, bringing all the

### <

100) silicon likeminima. down towards the

### <

111### >

minima. Measurements of the effects of hydrostatic pressure upon the threshold field in a### <

100 ~ direction at 77°1:revealed that it increased with increasing pl'essure(49).

The souroe of the

### N.D.C.

in n- Ge has been the subject of some debato.In theil' initial paper reporting observation of micro-wave omission from n - Ge, McGroddyet al (44) and subsequently Chang and Ruch(46) and

between <111> and <100> minima as the source of the N.D.C. Later work by IIIeltz and I1CGroddy(49)would seem to undermine this model since

their hydrostatic pressure measurecents indicated that, as the

### <

100> and~111> minima approach each other, the threshold electric field increar,cs. A simple model of the transferred electron effect would sugeest a decreaso of threshold electric field as the valleys approach eaoh other.

An alternative model suggested by Dumke(51) relies only upon

non-parabo1icity of the individual

### <

111> minima. In this calculation electrons were allowed to rise to quite hieh enercies within the### <

111### >

minima, as a consequence of the omission of the### <

100) minima which provict.:3 an enerGY ceiling. Dumkefinds that non-parabolicity alone can provicle an N.D.C. which arises from the increase of the effective mass with enerGY.The introduction of an N.D.C. by application of a ID1iaxial stress in Smithts(48) Vlork, on the other hand, is attributed to transfer between

the now non -equivalent

### <

111> minima. Clearly, however, sinoe an N.D.C. is known to exist in the absence of uniaxial stress for current flow in a (100) direction, this latter model is a gross simplification of a verycomplex situation.

In a very recent LIonte Carlo calculation, Fawcett end Paiee (52)

have been able to account for nearly all the observed behaviour by

suitable choice of the various disposable parameters. However, beoauoe

the final behaviour is a consequence of the interplay of a number of similarly small effects a detailed intuitive explanation remains complex.

Thus, in SUItlLlary,in 1969 N.D.C. VIasknown to exis·~ in n - Oe

*for* current flow parallel to the

### <

100)" direction, and for temperatu.res below 150oK. The magnd.tude of the negative slope mobility had,however, not been measured at 71°K(44)

### *

and the threshold field was variously reported as 2.2 KV/cmand 3 KV/cm(45).### ---*

It has alrea~ been pointed out that the measurement by ChanGand Ruch has been discounted by the authors, for in presenting their

result at this temperature they poir~ out that the measured neeative

Refe!'ences

1. J. Eok and P. Uozieres

J. Phys.Chem.Sol.'~, 707-714 (1963)

or

A. C. Baynham and P. W. Braddock

Sol.Stat.Co~.

*l,*

371 (1966)
2. D. J. Bartelirik
Phys.Rev.Lett.

### 12,

510-513 (1966)or

Pbys.Rev.lll, 1101-1124 (1970)

3. O. Holte!'

Phys.Rev.

### m,

No.6, 2548-2553 (15 ~,!a!'ch63) 4. D. Eohm, E. P. Gross?bys.Rev.

### 12,

No.12, 1851-1864 and 1864-1816(June 15, 1949)### 5.

G. A. Swartz and B. B. RobinsonAppl.Phys.Lett.2, 232-235 (1966)

B. B. Robinson and G. A. Swartz, IBIl.

J. Res. and Dev.ll, 601-606 (1969)

6. E. Schlomann

J.A.P. ~, No.3, 1422-1424 (March 69)

7. A. R. Hutson, J. M. McFee and D. L. ;'lhite

Phys.Rev.Lett.l, 237-239 (1961)

Phys.Rev.138, 6A, 1121-6 (June 65) 8.J. E. Gunn

9. H. J. Stocker

### j],

110.26, Phys.Rev.Lett. (26 June 1961)9a. P. N. Butcher - Private Communication

-21-10. T. A. Midford and H. C. Bowers

Proc.Inst.Elect.Electron.&1grs. ~, 1724-1725 (1968) 11. P. N. Robinson, G. S. Kino ruldB. Fay

~ETrans.El.Dev. 612-615 (Sept 1967) 12. W. Frey, R. ':1. H. Engelmann and B. G. Basch

Proc, 110GAConf. (1970)

13. P. Kozdon and P. U. Robson Proc.Moga. Conf. (1970)

14. J. Koyamo, S. O'Hara, S. Kawazura and K. l!~~abe S.S.Device Conference Boulder (1968) 15. B. K. Ridley and T. B. \7atkins

Proc.?hys.Soc.

*lQ,*

*293-304 (1961)*16. C. Hilsurn

Proc.I.R.E.

### 2£,

185-189 (1962)11. J. B. Gunn

I.B.M. J.Res.Devel. ~, 141-159 (1964)

-22-18. I. B. Bott and W. Fawcett

Advances in Microwaves,

### .l,

223-299 (1968) 19. C. Hilsum,Proc.7th Intern.Conf.Phya.Semicond. Paris, 1127-1139, Donod, Paris 1964.

20. As 19, or

A. R. Hutson, A. Jayaraman and A. S. Cariell Phys.Rev.

### 122,

786-796 (1967)21. As 18. 22. As 17, or

### 24.

J. \'1. Allen, M. Shyam, Y. S. Chen, G. L. Pearson### 25.

J.### W.

Allen,### M.

Shyam and### G. L.

Pearson, Appl. Phys.Letters,### 2,

### 39-41

(1966)### 26.

C. Hilsurn and H. D. ReesElect.Lett. ~,

### 211-218 (1910)

### 21.

As### 19.

and### 20.

21s. J. L. :Birman, lI. Lax and R. Loudon Phys.Rev. ~,

### 620-622 (1966)

### 28.

E. G. S. PaiseProg. in Semiconductors, ~,

### (1964)

### 29.

lr.Frohlich and V. B. PsranjapeProc.Phys. Soc. B69,

### 21-32 (1951)

### 30.

T. KurosawaProc.Int.Conf.Phys.Semicond. Kyoto

### (1966)

or J.Phys.Soc.Jap.Suppl.### 11,

### 424 (1966)

### 31.

W. Fawcett, A. D. :Boardman and S. SwainJ.Phys.Chem.Sol. ~,

### 1963-1990 (1910)

### 32.

J. G. Ruch and G. S. KinoAppl.Phys.Letters

### 12,

### 40-42 (1961)

### 33.

J.:B. Gunn and :B. J. ElliottPhys.Letters

### g,

### 369-312 (1966)

### 34.

### w.

ShockleyBell System Tech. Int.

### ll,

### 199-826 (1954)

### 35.

H. KroemorProc,

### IFlE.2.l,

### 1246 (1965)

### -23-36.

D. E. McCumber and A. G. Chynoweth~rans.El.Devices ED-13,

### 4-21 (1966)

### 31.

### s.

M. 1~ahrous and P. N. Robson38. 13. K. Ridley

Proc.Phys.Soc. ~, 954-966 (1963)

39. E. Kroemer

IEleTrans. e1. Dev. ED-13, 27-40 (1966)

40. P. N. Eutcher

Phys.Lett.

### 12,

546-547 (1965)41. J. 13. Gunn

Proe.7th Int.Conf.Phys.Semicond. (Plasma effects)

Paris 1964, 199-207 ~~od 1964.

42. J. S. Heeks

~Trans.el.Dev. ED-13, 68-79 (1966)

!DU, Jnl. or Res. and Dev •

### .1.1,

337 (1967) 45. E. J. Elliott, J. E. G\U'U1,J. C. I.IcGroddyAppl.Phys.Lett.

### 11,

No.8, 253-255 (15 Oct 1967)45a.

### J.

D. Gur~ and 13.### J.

ElliottPhys.Lett.

### gg,

No.4, 369 (1 Sept 1966) 43. H. W. ThimProc, ~~ ..2.5" 446-447 (1967) 44. J.

### c.

r.!eGroddyand U. I. UathanAppl.Phys.Lett.11, 111-112 (1968) 45b. J. G. Ruch and G. S. Kino

Appl.Phys.Lett. ~, 40 (1967)

46. D. U. Chang and J. G. Ruch

41. As 45b.

48. J. E. Smith (Jr.), J. C. llcGroddy and M.I. nathan Electron.Device Conference Boulder, 1968

IBM. Report, Rc 1013 (Feb 14, 1968) 49. P. J. :r.:elzand J. C. !~cGroddy

-24-Electronics Letters

*1,*

Ho.11 (Nov.1967)
50. W. Fawcett and E. G. S. Paige
51. W. P. Dumke

Phys.Rev. ~, 987-996 (1970)

52. W. Fawcett and E. G. S. PaiGe

J. of Phys. C. ~, 1801 (Sept.1971)

53. A. P. Ueukerman and G. S. Kino

10th Int.Conf.Pbys. of Semicond. 40-45 (1970)

E.

*o.*

S. Paige
I.B.ll. Jul. of Res. and Dev.

### 1l,

No.5, 562-567 (1969) A. C. Baynham,I.B.t!. Jul. of Res. and Dev•

### .u.,

No.5, 568-572 (1969) A. C. BaynhamElectronics Letters,

### ,2"

no.10 (1970)-25-2. Vll'l.veProp:?cation in Conductinr~ Media

:) It was proposed in Section 1 that amplification may be achieved by launching a (quasi) T.E.!!. wave through a negative resistance modium. In the absence of any materials having a total negative resistance, it was suggested that materials which exhibit negative differential conductivity could possibly be employed, if biased into the reeion of N.D.C. as shown schematically in Figure 1 of Section 1.

In this section we examine this proposed amnlification rroc~

and the ideas developed here form a basis for the remainder of the work to be described. We deal first with wave propagation in an infinite uniform medium, then introduce successively, complexities arising from finite specimen geometry, non-uniformity, anisotropy, and

frequency dependence of the negative resistance process. Each of these features will be seen to place its oVln constraints upon any experimental system designed to observe wave amplification in a N.D.C. medium.

Consequently whenever a new observational system is introduced, in subsequent sections, the conditions established here will be relied upon in the choice of the experimental parameters.

### -26-I

~i

II

### I

!

### i

I

### I

2.1 T.E.!i. 'j'lavePro!'~ea.tionin an Infinite Uniform Hedium From Ma.xwell's equations Vie have

where electric and magnetic field vectors are E and H respectively,

### -

*-l*

is the current density *Po'*

the permeability of free space (which is
relevant in all cases of present interest) and t is time.

### 'Y'/\

and### Y.

are the vector operators curl and diVe respectively.Assuming that the wave is transverse electric, i.e. tha.t the electric vector lies in, for example, the x direction, which is

### *

orthogonal to the direction of wave propaGation, z, we obtain

whel'e ~ and ~ L are the conductivity and lattice dielectric constant tensors. These will be asswned to be diagonal and time independent

### *

•If the wave has the form

### ! -

### 1lo

er.>### [1

(c.;t - kz ~then

i.e. _{• •} _{•}

NOVl, both the conductivity *(Y,* and the wave number k are in

### *

These assumptions imply that

### SZ.!J. ..

### fa

o. The material is thus implicitly assumed to be free from space charge accumulation.'s

-27-general complex, allowing respectively for a current which leGs the electric field, and daopine of the wave. By writing

(]la <r'R+i"i

• •

### •

In (1) and separating real and imaginary parts \'Iefind that, from

_ 11\

### )2

+v

**1-**

### +-e

C2o

The positive sign must be taken so that

where ~ is the real wave vector arising in the absence of all the free carriers, i.e. k

### e

1/2 ~LR· L 0

of equation (1) we also have

*_ c:* k2

R 0

a

### 2e

*oW*

### 1<R

### •

•### •

Using the imaginary part

Hence,using

### (3),

k .•

l.

-28-Use of the follo'wing identity

~2

R

### (~1

*I(p*

*+*

### r

+ ~### ))

a:_{~}

_{-}

_{<>i}

_{on}

+ +

### -

### €

LE o0J €LE.oUl_{€~}

_{€~}

_{CA.>}

_{2}

allows us to write

### .

### ~{

<Y.### +

### /~1

### o;_

### )

2 2 1/2

~

~R )}

k ..._{1}

### f2

_{--}+ 1 +

_{+}

_{EL foOl}+

_{222}

eLf-oW

2 _{€} _{E.} CA)

L 0

• •

### •

(5)The lower sign must be taken here

The basic characteristic of T.E. wave propagation in an infinite uniform medium are specified by equations (3) and (5) for the complex wave number, and equation (4) which relates the signs of ~ and ki•

It is the latter equation which provides the basis for the gau1 process. ITe see that, as the real conductivity goes from positive to neGative, the relative signs of ~ and ki change. Since loss is known to occur inthe everyday world of positive resistance media, gain must be

assooiated with a negative conductivity; a conclusion which is bon1o out by equation (4), fol' if

### kR;>

0, ~### <

0 then ki### >

0 andthe wave asoumes the form

We note furtheI' that theI'e is no dal"!1pingof the wave when there is zero real conductivity, whilst the real pD.rt of the wave vector tends to the lattioe limited value.

### -29-.

<7' o N### -

### --_

....### -

### ---

### -

### ----_-...

...### _

-0·2### ---•

_{I}

### I

### I

### I

### I

### I

### I

### I

### I

### I

### I

### I

V### I

### I

### I

### I

### I

### --T---~

### I

### I

### I

### I

-,-_.---~ tu :::> VI VI FIG. ISCHEMATIC DIAGRAM OF RADIATION INCIDENT· UPON A FABRY

PEROT COMPOSED OF NEGATIVE RESISTANCE MATERIAL.

### z

0 0 II.. VI ::J ~ "0### i,

:-=.=.~~~ (tl , tJ ~ cl 0·8Q..

_{I}

.,._.--_-o, «

### t

Cl ~ 0·6 0:: -0 L<... V1 :r:: z u LLJt:: t- .

0- Z

--,

_{_..}

<:

0 :7:,

0'4

w ~

U. _{I} _{V1}

<

### '"

### .,_

**A-4** SHEET

_{}

### .__----o

0·' 0·2**__**

**._-_.-**

**---__**

**.--.---..__...**

-OJ 0·4 O'5 0·6 0·7 0·8 0·9 1·0

t----SPEClt",AN--~

SmGLE PASSS!GNALLEVEL MULTIPLE PASS SIGNAL LEVEL

Ct1S-"

RRjR3/02617

---2.2 Finite Snecimen Geometry

2.2.1 Fj.ni to Snoc:5.rnel1Geometry in the Direction of

1.7avePron(1f'ation

In this section we introduce a finite specimen Geometry in the propagation direction, as shown schematically in Figure 1.

It is ir.u:lediatelyclear that in the absence of gain we have a

",..

.Fabry Perot structure.

The amplitude of radiation, transmitted through a Fabry ",..

Perot etalon thickness A is

k.A 2 2k.A

Lt • Lo e 1 T (1 + 1'2e· 1 Cos (2

### ka

A) ••• )where Lo is the incident amplitude from the cavity's enviroTh~ental noise spectrum, for example and T and I' the surface transmission

and reflection coefficients. ~e now distinguish a number of distinct operational regimes for such a structure with potential internal gain.

(i) 1'2 e 2kiA< 1

If 1'2 e2kiA

### <::

1 , that is, there is no round trip gain in tho cavityL T2 kiA

L 0 e

t - --- _{•}

_{•}

_{•}

(6)
( 2 2k.A

1 - I' e 1 Cos

and transmitted signals remain finite, though under some cf.rcumst.ances

they may be larger than the incident signal. Th.e threshold for this insertion gain is olearly defined by

T2 _{e} k.A

1

... 1 ...

--~~:""'"!""-1 2 2 leA- I' e 1.

at the frequency of peak gain. L~sertion gain occurs then if

-30---.---~---.---.-~-~----...

• • •

This IIki! product" which defines the threshold for insertion eain is more usefully expressed as an "l~!product" usine equation (5) when the complex cond.uctivity

~.. ne

### (PR

+ i### P:t )

of the host negative resista.."'lcematel'ia.lis mown. The

(free ca.rrier concentration x A) pl.'oduct(IrA product) is employed in describine the stability of a specimen, and will be used

### *

extensively throughout the remainder of this work •

The surface reflection and trensmission coefficients m~y,
of course, be expressed in terms of the free spa.ce wave - vector
k_{o} and the comulex wave - vector within_{•} the material of tho
-Fabry Perot uSlllg Fresnel's equations. Thus the exact insert ion

gain L_ L*m/L L * is derived with the aid of equation (6)

~ lOO

and becomes

• 16 k/("'a 2 + ki2).-2 kiA/ {( 1 +*ol,.2)* (A12+ B2 +

### c

2 +### n

2)+ 2 (1 - d...2) (A1B + CD) + 2 ~ [(B2 - A12 + D2 - 02)C03

*cp*

+ 2 Sin

### cp

(:BC - A1D)] } • •• (8)### *

It should be pointed out that owing to the free carrier contributionto the surface reflection, and transmission coefficients the k.A 811d KA

l.

products defined by equation (7) are not truly constants. They show a dependence upon the free carrier concentration which is negliGible for lightly doped material. However, in more heavily doped material, o\"dnC to the laree free ca.l"riercontribution to rand T the HA product must bo treated with caution.

-31-afte~ some m~ni~ulation Vihe~e

B

### =

C a 2 k. k

:l A

D ...

The transmitted powe~ is therefore d.etermined by the pa~a.meters1<:,...

.1.\

Through equations (3) and (5), it can be

expressed in terms of ko' A , the f~ee carrier concent~ation cnd . complex mobility.

At a later stage the insertion gain is computed for both

n - Ge and GaAs as a function of free carrier concentration uzine

these equations. The p~osramme written for this purpose is eiven in Appendix 1.

We have seen that when there is no round trip gain within the cavity, the device may exhibit either insertionIDss or

insertion gain. In the latte~ case, the bandwidth of the amplifier is determined by the magl'litude of the internal ~enection coefficient, or, in other wcrds by the strength of the feedback process,

Equation (6) indicates that the transmitted sicnal falls to

### 1 / {2

of its peak amplitud.e when*{ V2*

r2 e2 kiA _ 0.4 }
r2 e2 kiA
k

*s:*

### ..1.

Cos-1r' 2A

Hence, remembering that at present we specify no round trip cain

within the c<?vity, the bandwidth is, (in tems of the real wave vector)

(ii) 1'2

### ---{ Y.- ;

Cos-12k.A 1

### ~ =

• 2

'~k

==-r ~Athen equation (6) becomes inv2.lid whenever Cos (2 ~A) ... 1 as a sum of the multiply reflected waves

### ,.,

within the Fabry Perot etalon. The sumhas in fact become infinite, indicating the co~~encement of oscillation. The threshold for

oscillation is thus given by

• •

### •

(~Using eQuation (5) this kiA product can again be expressed as en l1Aproduct for a material of known complex mobility. Thus a second

nA product is defined which determines the threshold for oso i.ll.at f.on;
The analogy to the NL product widely used to c~efinG
the threshold of domain mode oscillation (Ut ~_{.,} le)_{osc} is clea,r:
The NAproduct defines the threshold of electromagnetic instability
transversa to the applied electric field, whilst the conventional
Nt product defines the threshold of space charge instability parallel

to the applied electric field. Once again we point out the:t this

second liA product defined in equation (a~ is only approximately a

constant, owing to the free carrier contribution to r.

AS6uminsthat the system does not saturate, then at the

frequencies for which the phase angle ~A ..

### ,

we see from (6)that infinite output is predicted. However an infinitessimally

removed frequency for 'which COS~2 l:nA) ia mareinally sma.ller then

### .

-33-unity has a finite transmitted amplitude. The width of the predicted spectral emission siGnal is then infinitely small, and

it is centred upon a normal mode of the Fabrey ptrot cavity. (iii) r2 92 kiA

### :>1

\'Jhen r2 e2 kiA

### >

1 , aecumdng that the system a,e~!.in(loos not saturate, for all those frequencies for which the productr2 e2 kiA Cos (2 kaA)~1 infinite transmission occurs. of this broad power spectrum will occur, as before, when

The e~es

2 2 k.A ( )

r e ~ Cos 2kaA a 1.

Any real system must of course reach an eq_uilibrium situation throueh some nonlinear process.

### In

this situation, the rate of supply and loss of microwave energy will have become equal ,ASSUr.ling that the rate of generation of power is still a maxdmum where the small signal condition Cos (2 kaA) - 1 is satisfied,

then the system reverts to that behaviour already ascribed to CUCll

a regime; that is to an infinitely narrow emission spectrum which is centred upon a cavity mode or modes.

In this section the conclusions have been drawn that a negative resistance amplifYll1g medium having boundaries in the direction of wave propagation may behave as

a) a circuit element havine net insertion loss

b) an amplifier havine a bandwidth determined by the product r2 e2 kiA, and a threshold defined by an NA product. c) an oscillator which has an infinitely narrow spectral

emission line centrod upon a normal mode of the cavity, end having a threshold defined by an NA product.

It is the object of the present work to observe each of these classes of electromagnetio instability.

-34-

>-o _{.-=}

·z

-CD CD .0

C) c:: CO

### ..

C)-CO >- CO >- Cl)

**.z=.** **It:** E .-= c::

u= _{6=}

:s!

CD CD.o .. .0

:c u co

### -

co### ..

co ti o

### -

.0co CD Cl) _{}

### >--

### ~.=

- c::en W.- J:

C") C") (W) (W)

### ...

### ...

### ...

### ...

0 0 0 0

r" r" .-

.-M M cwS cwS

### "

### "

"- Aco co co co

c:: c: c: c:

### ...

### ...

### ...

### ...

### ...

### ...

### ...

### ...

0 0 0 0

r"

### ...

### ...

### ...

### an

### an

iii iii### "

_{"}

_{"}

### "

### c

### c

### c

### c

>-~ ..J co « ~ en :2 U- C\I 0

en_{w} _{0}

en ·H

en rr..

c:(

..J

**________**

**Lfl**

### _@__Q_J_

**. ----.w**

**U**

**U**

I-Z

W 0:

0::

::>

### u

Finite Srec:i.nen Geomotry, in the Di:rection of

the Annlied. Electric Field.

The conclusions which have been reached in this section hnve, thus far, been of a general nature. However, it is now necessary 2.2.2

to draw conclusions which refer to the specifio type of neeative re::b',;;z:CG

process to be used.

### In

section 1, the transferred electron effect was introduoed as a mechanism providing a suitable neGativedifferential conductivity (lJ.D.C.) for the present experiments.

We envisage a system in which a DC electric field biases a sample into a region of N.D.C. Incident electromagnetic waves then senzo the negative slope conductivity and behave as if incident upon a lllatorial having a total negative resist~~ce as indicated in Figure 3.·

In Section 1, however, it was pointed out that a sample <")h1ch has a bulk N. D.C. became unstable to space charge fluotuations 'when biased into the N.D.C. range. This is clearly a complication which is to be avoided if possible, in order that experimental obeervat Lono

of the electromagnetic. instability may be clear cut. This choice 01

experimental regime stands in marked contrast to the large body

of work which has already been devoted to the N.D.C. prooess in Gn..t\s (see Figure 2); Vie choose to impose space charge ST.AJ3ILrryby makinc UL smaller than critical value for domain formation, and to oxt rac't microwave pOVier from the bulk N.D.C. by allowing electromagnetic

instability in its place i.e. by makine NA groater than the critical value for electroml?gnetic instability. In acldition to the tYIO foree;oing regimes in which microwave power may be extracted from

a sample having a bulk N.D.C. there is, of course, a third ono in which both space charge and electromagnetic instability are

simultaneously present. Two of these regimes, l'eeimes inwhich electromagnetic instability is operative, are now examined in more detail.

-35-Space charee stability is achieved most readily by imposing a low Nt product upon the specimen. Under these

circumstances, the specimen does not, however, aHsume a unifol'n1 spatial distribution of the biasine electrio field(1). !.;oreovcr, owing to both the electrio field dependence of the free oarrier oontribution to the total d.ielectrio constant(2) and the associated accumulation and depletion layers, any such non ~~i£ormity of biasL~2 eleotric field is reflected in a correspondingly non uniform

./

"microwave path length" within the Fabry Perot cavity. Thus, this spatially non-undf'crm biasing electric field is of clear importp.nce to the present work.

We calculate the spatial distribution of electric fie-Id and free carrier concentration neglecting diffusion. The onission of this tenn is justified ~ on the grounds that, in similar calculations, McCu;nber and Chynoweth (3) found it to be unimportant

everywhere except in regions of very rapid discontinuities, and *1"":...J.,_~.k*

beeeJls - ef the uncertainty which surrounds the precise form wh i.chth:i.:1

term should take(4).

The iterative procedure which we adopt commencos at a point adjacent to the metallic cathode contact. Here the semiconductor has an electron concentration which is approximately equal to thc.t

existing within the metal. For a chosen specimen current density

Jo' an electron drift velocity V, and field E1, may therefore be deduced. An arbitrarily small increment in electron drift velocity

### Rv

is then chosen in order to initia.te the iterative procedure. We look for a stationary solution for which\}

### _.

### -

J .. - -",### of

0~t